Structure determination of <i>A</i>~2~<i>M</i>^3+^TaO~6~ and <i>A</i>~2~<i>M</i>^3+^NbO~6~ ordered perovskites: octahedral tilting and pseudosymmetry
Barnes, Paris W.; Lufaso, Michael W.; Woodward, Patrick M.; Acta Crystallographica Section B 62 (2006) 384–396; doi:10.1107/S0108768106002448

data_2100513
_publ_section_title
;
 Structure determination of <i>A</i>~2~<i>M</i>^3+^TaO~6~ and
 <i>A</i>~2~<i>M</i>^3+^NbO~6~ ordered perovskites: octahedral tilting
 and pseudosymmetry
;
_journal_coeditor_code           WS5031
_journal_date_accepted           2006-01-19
_journal_date_recd_electronic    2005-06-10
_journal_issue                   3
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              384
_journal_page_last               396
_journal_paper_category          FA
_journal_paper_doi               10.1107/S0108768106002448
_journal_volume                  62
_journal_year                    2006
_chemical_formula_sum            'Al Ca2 Nb O6'
_chemical_formula_weight         296.04
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_audit_creation_method           'from EXP file using GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 89.970(4)
_cell_angle_gamma                90.0
_cell_formula_units_Z            2
_cell_length_a                   5.37706(9)
_cell_length_b                   5.41557(9)
_cell_length_c                   7.62550(13)
_cell_measurement_temperature    298
_cell_volume                     222.053(6)
_computing_structure_refinement  GSAS
_diffrn_ambient_temperature      298
_diffrn_measurement_device       BT-1
_diffrn_measurement_method       reactor
_diffrn_radiation_probe          neutron
_diffrn_radiation_source         NIST
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     1.5403
_exptl_crystal_density_diffrn    4.428
_refine_ls_goodness_of_fit_all   1.22
_refine_ls_matrix_type           full
_refine_ls_number_parameters     43
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.02
_refine_ls_shift/su_mean         0.01
_cod_data_source_file            ws5031.cif
_cod_data_source_block           Ca2AlNbO6
_cod_depositor_comments
;
The following automatic conversions were performed:
'_geom_bond_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (114
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (615 times).

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 

The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (114
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to /home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.1 from 2010-06-29 (615 times).

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        222.050(10)
_cod_original_sg_symbol_H-M      P21/n
_cod_database_code               2100513